Template-Free Electrochemical Growth of Single-Crystalline ...leung. 113...¢ ...
Click here to load reader
Embed Size (px)
Transcript of Template-Free Electrochemical Growth of Single-Crystalline ...leung. 113...¢ ...
Template-Free Electrochemical Growth of Single-Crystalline Zinc Nanowires at an Anomalously Low Temperature
Debabrata Pradhan, Shrey Sindhwani, and K. T. Leung* WATLab and Department of Chemistry, UniVersity of Waterloo, Waterloo, Ontario N2L 3G1, Canada
ReceiVed: July 01, 2009; ReVised Manuscript ReceiVed: August 11, 2009
Zinc nanowires of serpentine geometry have been grown on conducting plastic and glass substrates in an aqueous electrolyte at an anomalously low temperature of 0 °C by a one-step, template-free electrodeposition technique. These nanowires are of several micrometers long and with a diameter of 20-200 nm. These nanowires are also single-crystalline and found to be coated with a 5 nm thick ZnO shell with an epitaxial relationship to the Zn core.
Metallic nanowires are one of the important classes of nanomaterials with a wide range of technological applications.1,2
Of the several common growth methods for metallic nanowires, thermal evaporation and electrochemical deposition have been extensively used because of their simplicity and low-cost advantage. Unlike thermal evaporation that often requires a relatively high temperature (>500 °C) to prepare nanowires, electrodeposition is usually carried out at a considerably lower temperature, from room temperature to 90 °C, making it a more attractive technique for substrates with lower heat tolerance (e.g., polymers and plastics). In most cases, one or multiple metals are electrodeposited into a template, such as anodic aluminum oxide, which is subsequently dissolved in a solution to harvest the nanowires.3,4 More recently, Penner and co-workers have introduced new techniques to synthesize polycrystalline nanow- ires of several noble metals horizontally decorated on substrates by using either electrochemical step edge decoration or litho- graphically patterned nanowire electrodeposition.5 In the present work, we demonstrate, for the first time, the growth of single- crystalline metallic zinc (Zn) nanowires at an even lower temperature of 0 °C by a direct electrodeposition technique without using any template, thus making the synthesis not only a facile, one-step process but also appropriate for integration with biological materials. These nanowires could exhibit intrigu- ing properties, including metal-insulator transitions, one- dimensional superconductivity, and better performance in alkaline battery applications. For instance, Tian et al. have recently reported the unique superconducting behavior of Zn nanowires (obtained by an electrodeposition method using an anodic aluminum oxide template), while Heremans et al. characterized the magnetoresistance and thermopower of Zn nanowire composites (synthesized by thermal evaporation).6,7
To date, Zn nanowires have been primarily synthesized by using thermal evaporation,8 which involves evaporation of a Zn, ZnO, or ZnS precursor at 580-1400 °C and condensation to Zn nanowires in the colder region of the chamber (200-300 °C). Less popular methods such as spray pyrolysis,9 carbothermal reduction,10 cold-wall deposition,11 and ECR plasma deposition12
have also been used to produce Zn nanowires on a substrate at 150-300 °C. There are only a few reports of Zn nanowire formation by wet-chemistry techniques, such as hydrothermal synthesis at 150 °C,13 HF etching,14 and template-assisted electrodeposition at room temperature.15,16 The present work provides the first results of synthesizing single-crystalline Zn nanowires not only in a single step and without the use of template but also below room temperature. The formation of Zn nanowires at 0 °C demonstrated in the present work promises new opportunities in developing biologically active (“live”) nanocomposites,17 and applications requiring low-heat tolerant substrates such as low-cost plastics. Bacteria, viruses, and biomolecules have been shown to be capable of ordering inorganic nanocrystals into novel nanoarchitectures.18 As most viruses and biomolecules are known to become less stable above room temperature,19 there is great interest in developing this type of low-temperature growth procedure to allow in situ incorporation of “living” species into nanomaterials without the risk of denaturing.
In electrochemical synthesis, the types and concentrations of the electrolytes, the deposition potential, and the deposition temperature can all be used to control the structure, shape, size, and crystal quality of the Zn nanostructured materials.16,20 In most cases, a template is used to electrochemically synthesize a particular type of Zn nanostructures. For example, zinc inverted opals have been fabricated at room temperature using a polystyrene template,21 and in a very recent study, Gao et al. deposited zinc nanoparticles on indium tin oxide (ITO) coated glass at 70 °C via a metal-ligand-coordinated vesicle phase.22 In the present work, direct electrodeposition was carried out in a conventional three-electrode glass cell placed in a temperature bath held at 0 °C without use of any type of template. A Ag/ AgCl electrode was used as the reference, while a spiral platinum wire served as the counter electrode. The working electrode was either a In2O3/Au/Ag coated polyethylene tereph- thalate (PET) or an ITO coated glass substrate, with a resistance of e10 Ω. A CH Instruments 660A potentio/galvanostat electrochemical workstation was used to deposit the Zn nanow- ires with the deposition potential held at either -1.4 or -1.5 V (relative to the Ag/AgCl reference electrode), in an aqueous
* To whom correspondence should be addressed. E-mail: firstname.lastname@example.org.
10.1021/jp906198h CCC: $40.75 2009 American Chemical Society
Published on Web 08/17/2009
2009, 113, 15788–15791
9 | h
t 1 7,
9 | d
oi : 1
electrolyte solution of 0.1 M Zn(NO3)2 ·6H2O (Aldrich). The overall surface morphologies of electrodeposits were examined by a LEO FESEM 1530 field-emission scanning electron microscope (SEM). The glancing-incidence X-ray diffraction (GIXRD) data was collected by using a PANalytical X’Pert Pro MRD diffractometer with Cu KR radiation (1.54 Å) and an incidence angle of 0.3°. Transmission electron microscopy (TEM) measurements were performed using a JEOL 2010 transmission electron microscope with an operating accelerating voltage of 200 kV. The surface composition of the Zn nanowires was further analyzed by X-ray photoelectron spectroscopy (XPS) using a Thermo-VG Scientific ESCALab 250 Microprobe with a monochromatic Al KR source (1486.6 eV), capable of an energy resolution of 0.4-0.5 eV full width at half-maximum.
The SEM images shown in Figure 1 illustrate the morphol- ogies of Zn nanowires obtained by direct electrodeposition on a conducting In2O3-coated PET substrate at -1.4 V (with respect to a Ag/AgCl reference) in a 0.1 M Zn(NO3)2 ·6H2O electrolyte. Similar results were obtained with a deposition potential of -1.5 V. Evidently, entangled nanowires with sections of nonuniform diameters over the length (Figure 1b) are found to organize into fibrous globular agglomerations, shown in Figure 1a. These nanowires are several micrometers long, with the diameter in the range 20-200 nm (Figure 1c,d). These nanow- ires not only are curvy with a serpentine geometry but also show abrupt bending at various angles forming L-, V-, and multi- branch junctions (Figure 1c), as well as T- and Y-junctions (Figure 1d). While the origin of these junctions is unclear, we speculate that they could be related to the formation of defects and/or a secondary phase such as ZnO during growth. Zn nanowires with a similar entangled geometry have also been previously obtained on silicon, quartz, and alumina but at a considerably higher temperature range of 580-1225 °C by thermal evaporation.8 The present work therefore shows, for the first time, that growth of such Zn nanowires is possible even at 0 °C. If the deposition was carried out at room temperature without changing other deposition conditions, we obtained a porous film (not shown). Furthermore, the use of a less negative deposition potential (-1.0 to -1.3 V) also did not produce the observed nanowires. The use of higher electrolyte concentrations produced nonuniform films consisting of both nanowires and submicrometer-sized grains (0.5 µm). These results therefore suggest that the deposition temperature, potential, and electrolyte concentration all play a crucial and interdependent role in the formation of nanowires.
Figure 2 shows the corresponding GIXRD pattern of the electrodeposits on PET. The diffraction peaks can be indexed to the hexagonal crystal structure of Zn (space group P63/mmc)
with lattice constants a ) b ) 2.6637 Å and c ) 4.9430 Å, which are in good accord with the reference Zn lattice constants (a ) b ) 2.6650 Å and c ) 4.9570 Å, JCPDS file 01-087- 0713). It should be noted that, despite the use of the glancing- incidence mode for our XRD measurement, no diffraction peak attributable to ZnO is observed, suggesting that the nanowires consist primarily of Zn metal, and the concentration of any residual component such as ZnO, if present, is below the (bulk) detection limit of X-ray diffraction. Similar diffraction features can also be obtained from Zn nanowires in a conventional powder XRD measurement but with a considerably higher intensity due to a larger sam